Chemical Modification of Polymers with Flame-Retardant Compounds GIULIANA. TESORO C Fibers and Polymers Laboratories, Department of Mechanical Engineering, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139 I. Introduction ........................... ......................... 284 II. Definition of Terms .................... ...................... 285 A. Thermal Degradation and Combustion ...................... 286 B. Chemical Modification ............................................ 287 C. Polymer Flammability . . ................................... 287111. Scope of the Review . . . . A. Subject Matter.. ......................... . . . . . . . . 288 B. Classification of Subject Matter . . . . . . . . . 290 C. Selection of References ................... . . . . . . . . 290V. Flame Retardation and Flame Retardants in Polymers A. Principles . . . ......................... 293 B. Flame-Retardant Compounds . . . . . . . . . . . . . C. Chemical Modification with Flame Retardants ....................... 296 D. Evaluation of Flame Retardants . . . . . . . . . . . . . . . . . . . 298VI. Problems in Polymer Modification with Flame Re A. Incorporation of Effective Amounts . . . . . . . . . . . . C. Environmental ............................ ................... 301 D. Cost . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . E. Flammability, Smoke Evolution, and Toxicity of Combustion Products ...................................................W. Polymers and Applications ............................................. 302VIII. Wood, Board, and Paper . ......................... 304 A. Wood Products . . . . . ......................... 305IX. Fibers and Fabrics ....... ......................... 308 1. Introduction .... 3. Other Cellulosic Fibers . ......... 4. Regenerated Cellulose (R ............................. 317Journal of Polymer Science: Macromolecular Reviews, Vol. 13,283-353 (1978)@ 1978 by John Wiley & Sons, Inc. OO76-2083/78/0013-0283$01 .OO
284 TESORO G. Polyvinyl Chloride and Polyvinylidene Chloride Fibers ................ 323 H. Polyoleiin Fibers ................................................. 323 I. Specialty Fibers .................................................. 323 J . Fiber Blends .................................................... 324X . Plastics .............................................................. 325 A . Thermoplastic Resins ............................................. 325 1 . Polyolefins ................................................... 326 2. Styrene Polymers ............................................. 328 3. Polyvinyl Chloride and Related Polymers ........................ 329 4. Acrylic Plastics .............................................. 333 5 . Nylons ...................................................... 334 6. Linear Polyesters ............................................. 335 7. Cellulosics ................................................... 335 8. Polyacetals ................................................... 335 9. Polycarbonates ............................................... 335 10. Polyaryl Ethers ................................................ 336 B . Thermosetting Resins ............................................. 336 1. Phenolic Resins ............................................... 336 2. Amino Resins (Urea-Formaldehyde, Melamine-Formaldehyde Resins) ....................................................... 337 3. Unsaturated Polyesters Resins (and Alkyds) ...................... 337 4 . Epoxy Resins ................................................. 339 5. Polyurethanes ................................................ 339XI. Foams (Cellular Plastics) .............................................. 340 A . RigidFoams ..................................................... 340 1 . Polyurethane Foams .......................................... 341 2. Polystyrene Foams ............................................ 344 3. Other Rigid Foams ........................................... 344 B. Flexible Foams .................................................... 345XI1. Elastomers ........................................................... 345X 1 . Coatings ........................................................... I1 347 A . Nonintumescent Coatings ......................................... 348 B. Intumescent Coatings ............................................. 348References ................................................................ 349 I . INTRODUCTION The science and technology of synthetic polymers has undergone explosivegrowth in the last few decades. and the number of different polymeric ma- .terials in our built environment increases almost daily All organic polymersburn. and thus entail some measure of fire hazard in some situations. Withincreasing awareness of the nation’s fire problem (Report of the President’sCommission on Fire Prevention and Control. America Burning. 1973). ithas become evident that the problems associated with flammability of poly-meric materials must be attacked-and solved. With the large number ofpolymers in commercial use. problems of flammability and fire retardationare complex and multifaceted . Tables I and I1 indicate types and volumes of fibers and plastics producedin the U.S. To substitute polymers with improved fire performance. whererequired. either thermally stable new polymers of satisfactory performance
CHEMICAL MODIFICATION OF POLYMERS 285 TABLE I U.S. Man-made Fiber Production in 1973 Fiber B i l l i o n Pounds Rayon 0.89 Acetate 0.46 Nylon 2.18 Polyester 2.77 Olefin 0.42 Acrylic 0.74 Glass 0.69 Other 0.13 Cottonb 3.65 Wool 0.17Source: Textile Organon, Jan.-Feb. 1974, Textile Economics Bureau, Inc., New York.*Source: U.S.D.A. Economic and Statistical Analysis Division in Textile Highlights, De- cember 1973, American Textile Manufacturers Institute, Inc., Washington, D.C.properties have to be developed, or existing polymers must be modified byaddition of fire-retardant compounds. The latter, short-range approach, ismore important, technologically and commercially, at this time. Modification of known polymers may involve either a coating applied tothe surface of the material, or the incorporation of a fire-retardant com-ponent into its bulk at an appropriate stage of manufacture. During the last few years, many new concepts relating to flammability andfire retardants in polymers have evolved from research investigations ingovernment, university, and industrial groups. Much progress has been madein the development of principles, hypotheses, materials, and methodology.These technical accomplishments, stimulated in part by the pressure oflegislative action, and by new standards for flammability performance in use,in many instances have included short-range, pragmatic solutions to prob-lems which were not adequately understood or defined. Much work remainsto be done, much is being done, and the state of the art in this field of chemi-cal technology is a rapidly changing one. I . DEFINITION OF TERMS I Lack of precision in the use of terms related to polymer flammability, pol-ymer combustion, etc., has been noted by several authors (Miller, 1973;
286 TESORO TABLE I1 Plastics Sales in the U.S. for 1973 and 1974* Materia 1 1973 1974 Acrylic 233 243 Alkyda 334 388 Cellulosics 77 76 Coumarone-indene a n d petroleum r e s i n s 1 60 160 EPOXY 102 106 Nylon 87 88 Phenolic 624 587 P o ly e s t e r 468 425 Polyethylene, high density 1,248 1.275 Polyethylene, low density 2,691 2,769 Polypropylene 1,012 1,061 P o l y s t y r e n e and s t y r e n e copolymers 2,356 2,328 Polyurethane 593 622 P o l y v i n y l c 5 l o r i d e and copolymers 2,151 2,180 Other vinyls 390 420 Urea and melamine 488 475 Others b 138 147 Total 13,152 13,350*In metric tons x lo3. Source: Modern Plastics, Jan., 1975.aIncludes captive consumption, about 50%.bIncludes polyacetal, polybutylene, fluoroplastics, polycarbonate, silicones, thermoplastic polyesters, thermoplastic urethanes, and others.Nelson et al., 1974). Some efforts are currently underway to define andstandardize the use of terms and to produce a glossary with definitions inseveral languages. Until these definitions are decided on, and utilizing suchworking documents as have been produced by task forces and committeesin the course of these efforts,*t terms used in this review are defined in thissection in the hope that ambiguity and misunderstanding will be avoided. A. Thermal Degradation and CombustionThermal degradation. Irreversible chemical decomposition due to increase in temperature.* See Textile World, June 1975, pp. 107, 109.t Glossary in preparation by the Ad Hoc Committee on fire safety aspects of polymericmaterials, National Materials Advisory Board, National Academy of Sciences.
CHEMICAL MODIFICATION OF POLYMERS 287Pyrolysis. Irreversible chemical decomposition due to increase in temperature without oxidation.Combustion. Self-catalyzed exothermic reaction involving two reactants (fuel and oxidizer).Fire. Uncontrolled combustion.Flames. Gas-phase combustion processes with emission of visible light.Ignition. Initiation of combustion.To Glow. To burn without flame, but with visible light. B. Chemical ModificationComonomer. Compound added in polymer synthesis and becoming a part of the polymer molecule.Additive. Compound added after the polymer has been synthesized but before or during its conversion to final form (e.g., fiber, plastic); not covalently bound to polymer substrate.Finish. Compound or combination of compounds added after conversion to end product (e.g., fiber, fabric). May be covalently bound or deposited.Effectiveness. Ability of flame retardant to decrease flammability of the poly- mer substrate in which it is present.Synergism. Observed effectiveness of combinations of compounds greater than the sum of the effects of individual components.Antagonism. Observed effectiveness of combinations of compounds smaller than the sum of the effects of individual components. C. Polymer FlammabilityAfterglow. Glowing combustion in a material after cessation (natural or induced) of flaming.Autoignition. Spontaneous ignition of a material in air.To Char. To form more or less pure carbon during pyrolysis or incomplete combustion.Ease of Extinguishment. Relative facility with which a given material, once burning, can be extinguished.Ease of Ignition. Measure of the time or temperature at which sustained flam- ing of a material in air occurs (with reference to material dimensions and density, incident heat flux and air composition, temperature and velocity).Fire Resistance. Capacity of a material or structure to withstand fire without losing its functional properties.Flame Resistance. Property in a material of exhibiting reduced flammability.Flame Propagation. Spread of flame from region to region in a combustible material (burning velocity = rate of flame propagation).Flame Retardant. Chemical compound capable of imparting flame resistance to (reducing flammability of) a material to which it is added.Flammability. Tendency of a material to burn with a flame.
288 TESOROGlowing combustion, Oxidation of solid material with light, but without visi- ble flame.Self-extinguishing. Incapable of sustained combustion in air after removal of external heat or flame (with reference to material dimensions, orienta- tion and ignition).Smoldering. Combustion without flame, but usually with incandescence and smoke.Smoke. Fine dispersion in air of particles of carbon and other solids and liquids resulting from incomplete combustion.Toxicity. Harmful effect on a biological system caused by a chemical or phys- ical agent. D. Test Procedures(Limiting)oxygen index. Minimum percent oxygen in the environment which sustains burning under specified test conditions.Vertical, horizontal, 45" [test].Orientation of the test specimen during flam- mability test under specified conditions.Self-extinguishing. Does not continue to burn under the specified test con- ditions after the source of ignition is removed (under specified test con- di tions).FIame spread. Extent of propagation of flame in space or over specimen surface under specified test conditions.Char length. Length of totally or partly burned material after exposure of a specimen to a flame (under specified test conditions).Rate of heat release. Amount of heat released per unit time by specimen burning under specified test conditions. m. SCOPE OF THE REVIEW A. Subject Matter The technical literature covering various aspects of polymer flammability,of flame-retardant compounds for polymers, and of possible improvementsin the fire safety of our environment has undergone explosive growth in thelast decade. Many review articles, books, and conference proceedings haverecorded and reviewed scientific and/or technological developments in variousways. One might therefore question the usefulness of yet another review of thisimportant and growing field. However, the subject matter is so vast, in-herently interdisciplinary, and complex, that each review inevitably presentsa limited treatment, motivated by the specialized knowledge and approach ofthe author, and therefore primarily of value to those having similar interestsand research goals. The present article is no exception. It addresses primarilyconcepts in the chemical technology of flame retardation of polymers-andit attempts to review problems, approaches, and state of the art for this seg-
CHEMICAL MODIFICATION OF POLYMERS 289ment of the problem. Even with this limitation, a systematic and comprehen-sive coverage of the subject matter is difficult. On one hand, the molecularstructure of the polymers and of the flame retardants are essential considera-tions in discussing the thermal degradation and combustion of specific poly-mer/flame-retardant systems. On the other hand, the application or end-use ofa specific polymer (e.g., fiber vs. plastic) is an overriding consideration in thedefinition of all the properties required, including those which are affected bythe presence of flame retardants. In an attempt to acknowledge and discussthese two levels of systematic classification of the subject matter, this reviewcovers polymers in six broad technological (or application) categories (wood,fibers and fabrics, plastics, cellular plastics and foams, elastomers, and coat-ings) and, within each category, the chemical types of major importance. Thiswill allow discussion of specific problems of flammability and flame retarda-tion of the polymer in terms of its molecular structure and its application.Polymers covered in this review are those which exhibit moderate or low ther-mal stability, and undergo thermal degradation when exposed to temperaturesof below about 300°C for brief periods, even in the absence of an oxidativeenvironment. Although the mechanism of pyrolysis and thermal degradationof polymers differs for specific macromolecules, most known natural andsynthetic polymers are not thermally stable in this temperature range (Mador-sky, 1964): the subject matter discussed here thus includes an overwhelmingproportion of the commercial polymers of the 1970s. This review does not include discussion of high-temperature resistantorganic polymers in which thermal stability of the macromolecule is anintrinsic structural feature, generally attained by incorporating thermallyunreactive ring structures in the polymer chain. These polymers can preserve their structural integrity and retain usefulproperties over long periods of time at temperatures of about 300°C, or forbrief periods at temperatures approaching 1000°C (Nelson et al., 1974). Theprinciples used in the synthesis of thermally stable polymers have been sur-veyed in several recent reviews and monographs (Frazer, 1968; Jones et al.,1970; Black, 1970; Van Krevelen, 1975), to which the interested reader isreferred. While these materials currently represent a category of “high-per-formance” or “specialty” polymers which are available in limited quantities,and are costly, their availability and commercial importance could increaseat a rapid rate with increasing awareness of the improved fire safety they mayoffer in specific end-uses. In defining the scope of this review, it is important to point out that noattempt has been made to list and discuss the numerous test methods whichhave been proposed for the evaluation of polymer flammability in the labora-tory, and in simulations of fire accidents on various scales. The methodologyof testing for polymer flammability, the significance of test results, and theircorrelation with fire hazard form a complex subject which is beyond the scopeof this review, and best discussed by physicists and engineers. However,polymer flammability is not an intrinsic property of the material and thebehavior of a given polymer or material in relation to fire stress can be de-
TESOROscribed in quantitative terms only with reference to specific test methods orevaluation procedures. Some conceptual problems associated with flammabil-ity testing of polymers have been reviewed (Steingiser, 1972; Meisters, 1975).Generally speaking, however, test methods for flammability are designed withreference to a particular application of the material, and test methods pro-posed for specific applications (e.g., textiles) have been reviewed in this vein(Benisek, 1975). Notwithstanding the usefulness of these reviews, they donot generally provide an adequate background for discussion of polymerflammability in definitive terms, and descriptive, or qualifying terminologymust be used. In the review which follows an effort will be made to specifythe test method used (and to provide appropriate reference to it) wheneverthe effects of flame retardants on polymer flammability are discussed. When-ever possible, an indication of the significance of the test results reported willbe included. However, since the discussion will be generally limited to poly-mers and polymer/flame-retardant combinations evaluated by laboratorymethods, such indicationswill not necessarily be of value in assessing the prob-able or expected behavior of the polymers when used in practice, especially inconjunction with other materials. Knowledge of the flammability behaviorof a polymer in the laboratory is only the first step in the knowledge requiredfor the assessment of the flammability behavior of the polymer in use and,eventually, of the relative fire hazard posed by different polymers in realisticapplications. B. Classification of Subject Matter For the convenience of the reader in proceeding from the general to the spe-cific, the subject matter of this review has been classified (somewhat arbitra-rily) as follows. Sections IV-VII present a general background discussion and informationon the subjects of polymer degradation (IV), flame-retardant compounds (V),approaches and problems in chemical modification of polymers (VI), andpolymer applications where flame retardants and fire safety are considered tobe of interest (VII). SectionsVIII-XI11 discuss flame-retardantmodification for specific polymerapplications, namely, wood (VIII), fibers (IX), plastics (X), foams (XI), elas-tomers (XII), and coatings (XIII). The extent and depth of these discussionsvary greatly, reflecting both the relative importance of fire safety for the polymerapplication discussed, and the state of the art on modification of the specificproduct type with flame retardants. The emphasis placed on each polymer class within each section is, on theother hand, primarily a reflection of the current state of the art. C. Selection of References The selection of references of major scope and significance from the many
CHEMICAL MODIFICATION OF POLYMERS 29 1thousands which exist on the subject has been a major objective of this review.Critical selection can be a service to the reader, but inevitably entails theauthor’s judgment with regard to the relative importance of investigationsand technical publications. In making this judgment, the author has beenguided by the following assumptions and rationale: (1) Existing criticalreviews and books have been cited freely, indicating specific pages, sections,or compilations in the context of the discussion. (2) Literature referencescovering original investigations on some aspects of the subject have beencited when these were considered to be significant contributions to knowl-edge or technological development in the field. References to narrow, specif-ic, or procedural studies have not been included. (3) In the text, referencesto patent disclosures have been included only in those instances where a cor-responding literature reference was not available, and the material wasconsidered important. In other words, mere listing of patent disclosures hasbeen generally avoided in the text. References to patent disclosures are in-cluded in tabulations and summaries which show examples of flame-retardantcompounds, reactions, or processes. Cited patents in this case are intendedas illustrative, and will serve the reader as a starting point for searching rel-evant patent literature further. (4) Whenever possible, the first technicalpublication covering a specific concept or compound or process has been se-lected for citation. In most instances, this first disclosure of a new concept isfollowed by many elaborations, improvements, and variations which havenot been included in the bibliography, but can be found in most instancesin the cited reviews.IV. PYROLYSIS, THERMAL DEGRADATION, AND COMBUSTION The study of polymer combustion and of the means of retarding it (flameretardation) requires knowledge of thermal degradation, including pyrolysis(thermal degradation in an inert atmosphere), and thermal-oxidative degra-dation processes. These processes depend on polymer properties which areprimarily determined by molecular structure, and thus specific for each poly-mer type. Decomposition temperature, rate of thermal degradation underspecified conditions of heating and environment, composition of pyrolysisproducts and of the products of combustion depend on the chemical structureand composition, and are affected by the flame-retardant species present,and by other modifiers, if any. On the other hand, thermal degradation, igni-tion, and combustion processes for organic polymers can be represented sche-matically by the general sequences shown in Fig. 1 (p. 31 1) (Einhorn, 1971)with thermally induced decomposition clearly preceding ignition. Fundamental knowledge of the thermal degradation of organic polymershas been compiled in a classic book by Madorsky (1964), and more recentlydiscussed in monographs (Conley, 1970), symposia proceedings (Wall, 1973),and in an excellent review (Fristrom, 1974). The latter article includes a clear
292 TESORO TABLE III Examples of FlameRetardant Compounds Used as Comonomers Used in Applica- Compound f s) Polymer tion Reference CHz CH Ct 9. Polyacrylo- Fibers USP 3,487,058 nitrile (1969) C H ~ CE Br = Nark et al., 1968, VOl. 3, p. 199. Polyester Resins Stepniczka, 1976. (unsaturated) co Y Polyethylene Fiber8 I.P. Nelson, terephthalate 165th National Meeting, ACS, 6 Dallas, Texas (1973). (CZHSOIPCH~N(CHZCHZOH)Z Polyurethane Rigid USP (to I1 0 FO~UIS Stauffer Chem) 3,294,710 (1966), 3,235,517 (1966), 3,076,010 (1963).view of types of thermal decomposition, reaction regions in polymer com-bustion, solid-phase and gas-phase reactions as part of a generalized dis-cussion of fundamental concepts which arc essential for adequate understand-ing of flammability and flame retardation in polymers. The mechanism and the course of thermal degradation have been studiedextensively for specific polymers, particularly for cellulose. In the case of cel-lulose, considerable insight has been gained (Shafizadeh, 1968), and theeffectiveness of specific flame retardants can now be explained in the contextof a reasonable understanding of the mechanism of thermal degradation proc-esses (Hendrix et al., 1970; Walker, 1970). The thermal degradation ofpolyacrylonitrile and of copolymers of acrylonitrile has been the subject ofextensive investigations (Grassie et al., 1970-1973). A catalogue of the numerous studies of thermal degradation of specificpolymers and polymer compositions is beyond the scope of this review. It isappropriate to point out, however, that the thermoanalytical tools used toinvestigate thermal degradation in polymers have been greatly refined in
CHEMICAL MODIFICATION OF POLYMERS 293 TABLE IV Examples of Flame-RetardantCompounds Used as Additives Used in Applica- Compound (s) Polymer tion Reference syner- Cotton Little, 1947 gist for test halogenated fabrics, J. Kestler. Modern compounds coat- Plastics 44 (1), see ings, 102(1966), 47j9). Kuryla - Papa, 1973, poly- 96 (1970). ure- VOl. 1, thane pp. 133-194 foams - [ - ( C H Z ) ~ (CH)y-l Cellulose wood Canadian Patent I unsaturated alkyd resin 803,409 (1969), T o w a l . (1972). C. 9 polyester chlorinated coat- paraffin ings (BrCHZCHBr CHzO)3P=O Cellulose Fibers Tris-2.3-dibromopropyl acetate and phosphate triacetate y,o. ,%H7 Regenerated Fibers USP3,455,713 (1969). .PA celluloserecent years. Coupled with new, sensitive instrumentation for the analysisof degradation products, and of transient species in flames, these tools havebeen invaluable in providing needed understanding of thermal degradationprocesses and of the manner in which these are affected by flame retardants. V. FLAME RETARDATION AND FLAME RETARDANTS IN POLYMERS A. Principles Recent books on fire retardants (Kuryla and Papa, 1973, 1975; Lewin etal., 1975; Lyons, 1970a) include references and discussion on most com-pounds suggested as fire retardants for polymeric materials. These books alsosummarize present knowledge and speculation regarding the mode of actionof flame-retardant compounds, and current views, often controversial,regarding mechanisms of flame retardation in specific polymer systems. Gen-erally speaking, the flammability of polymers can be decreased either by al-
294 TESOROtering the products of thermal decomposition in such a way that the amountof nonflammable combustion products is increased at the expense of flam-mable volatiles (solid-phase retardation), or by inhibiting oxidation reactionsin the gas phase through trapping of free-radical species (gas-phase retarda-tion), or by a combination of these mechanisms. Most experimental obser-vations reported in the literature can be explained with reference to thesetwo mechanisms. Nevertheless, other modes of effectiveness of flame retard-ants play a role, at least in specific systems (Kuryla and Papa, 1973): (1)generation of noncombustible gases, which dilute the oxygen supply at thesurface of the burning polymer; (2) endothermic reactions of degradationproducts from the flame retardants with species present in the flame or sub-strate; (3) endothermic decomposition of the flame retardant; (4) formationof nonvolatile char or glassy film barrier, which minimizes diffusion of oxygento the polymer substrate and also reduces heat transfer from flame to polymersubstrate. The mechanisms of flame retardation outlined above do not contradicteach other, since several principles can simultaneously contribute to the ef-fectiveness or action of a particular flame-retardant system. Furthermore,combinations of flame-retardant species may be deliberately designed to in-clude several modes of action in a given polymer substrate: typically, com-binations of phosphorus and halogen are widely used, and it is postulated thatflame-retardant effectiveness of systems containing these elements includesa solid-phase effectiveness component (phosphorus) as well as vapor-phaseactivity (halogen). In considering combinations of flame retardants, it is also important topoint out the widely discussed but poorly understood phenomena of syner-gism. An excellent review of the subject is given by Weil in Kuryla and Papa(1975). As correctly pointed out by this author, the definition of synergisticeffect (namely, an observed effect of a combination of flame retardants which is greater than the sum of the effects of the components) is deceptively simple, and the term “synergist” has been frequently misused in the literature onflame retardants. Definitive proof of true synergistic interactions of flame re- tardants is not available, but a critical study of the literature suggests that the synergistic effects of halogen and antimony in polyesters (Pitts et al., 1970), of phosphorus and nitrogen in cellulose (Tesoro et al., 1968, 1969) are significant, while synergistic interactions of phosphorus and halogen are questionable, and apparent synergism of halogen compounds with peroxides and other free-radical-generating compounds in hydrocarbon polymers is almost certainly an artifact caused by reduced viscosity and dripping of the melt. B. Flame-Retardant Compounds Flame-retardant compounds, in order to be useful, must fulfill complexsets of requirements, many of which are specific for each product. In mostinstances, these requirements can be met only in part, and some tradeoffs
CHEMICAL MODIFICATION OF POLYMERS 295become necessary. In principle, in order to be seriously considered, a flameretardant added to a polymer should (1) reduce flammability as comparedto the unmodified polymer to a level specified for the product in terms ofproduct performance in a specificflammabilitytest; (2) reduce (or, at least, notincrease) smoke generation, under specified conditions of testing: (3) not in-crease the toxicity of combustion products from the modified polymer ascompared to the unmodified polymer; (4)be retained in the product throughnormal use (including exposure, cleaning, aging, etc.); and ( 5 ) have accept-able or minimal effect on other performance properties of the product in use(as established by relevant specifications). In addition, consideration must be given to the effects which the addedflame retardant may have on processing conditions, fabrication and costs inthe manufacture of the modified product, to health hazards which may resultfrom the presence of the compound in the work place, in the product, or inthe environment (industrial hygiene, physiological effects, and ecologicalconsiderations, respectively), and, of course, to availability and economics ofthe flame retardant itself. This formidable list of requirements readily explains why the number ofcommercially significant flame-retardant compounds is extremely small com-pared to the number of compounds which have been proposed and tested inthe laboratory, reported in the technical literature, and shelved due to failurein one or more critical properties. Flame-retardant compounds of value havebeen identified or discovered primarily by trial and error, rather than on thebasis of fundamental investigations of mechanism, or of systematic studiesrelating the parameters of molecular structure to flame-retardant effectiveness.The technology of flame-retardant compounds and flame-resistant polymericmaterials is well advanced, while scientific principles of flame retardantclassification are lacking. Known flame-retardantcompounds may be groupedas follows : (I) Inorganic acids and acid-forming salts (e.g., ammonium salts of sul-furic, sulfanic, phosphoric, hydrochloric, hydrobromic, and boric acid), whichact as dehydrating agents. These are solid-phase retardants, of importancewhere durability to leaching or washing is not required (e.g., wood, textilecellulose, and paper). (11) Inorganic salts which contribute to the formation of glassy coatingsaround the decomposing polymer mass (e.g., borates, phosphates, and sili-cates). (111) Inorganic salts and hydrates which decompose endothermically,releasing a noncombustible diluent (e.g., water) into the gas phase [e.g., -hydrated alumina (A1203 3H20)], of importance in specific applicationsof thermoplastic resins (e.g., carpet backings). (IV) Antimony compounds, which interact synergistically with halogen-containing flame retardants. The most important, antimony trioxide (Sb406)is extensively used in plastics and in fibers to reduce the amount of halogen-containing retardant needed, and thus minimize the effects of the modificationon performance properties.
296 TESORO (V) Organic compounds of phosphorus-generally solid-phase retard-ants-which are important for cellulosepolymers and polyurethane polymers.The organic moiety in these flame-retardant compounds contributes compat-ibility and/or reactivity with the substrate, while flame-retardant effectivenessand efficiency generally depend on the phosphorus content. (VI) Organic compounds of halogen-generally gas-phase retardants-important for hydrocarbon polymers and others. Effectiveness and efficiencydepend on the specific halogen (Cl vs. Br), on the halogen content, on thetemperature at which dehydrohalogenation of the compound occurs (thermalstability of the halogen compound, aliphatic vs. aromatic halogen) in relationto the temperature of decomposition of the polymer substrate, and on thepresence of synergists (e.g., antimony). (VII). Organic compounds containing both phosphorus and halogen. (VIII) Miscellaneous compounds which reportedly have shown effective-ness in specific substrate polymers under some conditions of measurement[e.g., tin, titanium, and chromium compounds (wool); molybdenum salts;zinc and magnesium chlorides (wood); and thiourea and ammonium thio-cyanate (nylon)]. C. Chemical Modification with Flame Retardants In the processing sequence of monomers to polymers, and, subsequently,to fibers, plastics, or other end products, flame retardants can be introducedin several ways. Each approach has advantages and limitations, which dependon many factors including processing requirements, properties of the flameretardants, level of flame resistance needed, critical product properties, etc. The approaches that may be considered are briefly outlined below. (1) Use of flame-retardant comonomers in polymer synthesis. The obviousadvantage of this approach is that the flame retardant becomes an integralpart of the polymer molecule, is resistant to leaching or removal, and thus toloss of effectiveness in use. The disadvantage resides in the effect of resultingchanges in the polymer structure on polymer properties including morphology(orientation, crystallinity, intermolecular forces) and mechanical behavior(tensile strength, recovery), as well as physical properties such as melting pointand glass-transition temperatures. The consequences of such effects are partic-ularly important in fibers. Comonomers have been used commercially asflame retardants in acrylic fibers, in polyester fibers, and in polyurethanefoams. (2) Use of flame-retardant additives in the polymer, such additives beingintroduced prior to spinning (fibers) or fabrication. This approach requiresthat the additive be stable under the conditions of spinning or fabrication,and that it be uniformly dispersed and retained in the polymer fluid duringprocessing in the amount needed to impart the desired level of flame re- sistance. In spite of these critical limitations, this approach is probably the most widely used for plastics (polyester resins, epoxy resins, etc.) and foams (polyurethanes). In the case of fibers, this approach has been used successfully
CHEMICAL MODIFICATION OF POLYMERS 297for regenerated cellulose fibers (rayon), and for acetate and triacetate fibers. (3) Graft copolymerization of flame-retardant monomers onto a preformedpolymer or fiber is a conceptually attractive approach to modification withflame retardants. It has been investigated extensively, and is reportedly ap-proaching commercial development for regenerated cellulose (rayon) fibersin Europe. While commercialization has not been reported, the flexibility ofthe approach and the multitude of disclosures in the technical literaturesuggest that this route may become more important in the future. (4) Finishing with flame-retardant compounds or systems is very importantin the case of textiles, which may be manufactured from one or more fibers.This is also obviously the only possible approach for the chemical modifica-tion of natural polymers (wood, cotton, and wool) with flame retardants.Flame-retardant finishes may be nondurable (removed in washing or cleaning)or durable (retained in washing or cleaning). In the latter instance, they mustbe insolubilized after applicaion, either by reaction with the substrate or bypolymerization in situ. Treatment with durable flame-retardant finishes hasfound successful commercial application for flame-resistant cotton fabrics. Finishing of textiles (fabrics) in principle would include graft copolymeri-zation with flame-retardant monomers, see (3) above, carried out as a topicaltreatment at the end of the fabric manufacturing process. The advantage offinishing as an approach is that it is versatile, flexible, and often relatively easyto implement in conventional equipment. However, the amounts of finishneeded are frequently large enough to impair product properties, and theapproach is by no means universal. ( 5 ) The use of flame-retardant coatings to protect flammable substrates isan old approach to flame retardation, still widely practiced (e.g., marine TABLE V Examples of Flame-Retardant Compounds Proposed as Monomers for Graft Copolymer Preparation Compound ( s ) References Manufacturer CHz = CHPOc(OCHzCH2CE) z USP 3,822,327 Stauffer Chemical (1974) Company CHI = CH Br , CH2 = CHCE ---- Ethyl Corporation BrCH2CHBr6H2OC I1 - CH = CH2 USP 2,993,033 Great Lakes Chemical 0 Corporation CHz = CHCOCH,P (0) (OR)2 German Patent a 1,100,287 (1961) Chem. Abst. 56, 7520 (1962) Chem. Abst. 63, 13420 (1965)
298 TESOROpaints). Flame-retardant coating formulations may be of the “conventional”(i.e., nonintumescent) or intumescent type, the latter type being more effec-tive, technologically advanced, and costly. In flame-retardant coatings, agingand weathering characteristics are critical, and not easily attained. Examples of flame-retardant compounds of each of the types outlinedabove are summarized in Tables 111-VII. TABLE VI Examples of Flame-Retardant Compounds U e as Durable sd Finishes on Fabrics Fiber App 1ica- Compound ( s 1 (polymer1 tion Reference I ( H O C H ~k ~ + ~ c ~ - ) Cellulose Cotton Lyons, 1970a, pp. + -Nn2 containing 189-208. coreactants Cotton Aenishanslin, Text. Res. J. 2, 375 (19691, lJSP3,423,369(1969). Ce 1lulose Cotton Eisenberg and Weil, Text-Chem. Col. 5 , 180 (19741, USP 3,69 5,925 ( 1972 1. (BrCH2CHBrCH20) aP=O Polyethyl- Polyester ene- tereph- thalate Titanium and Keratin woo1 British Patent Zirconium complexes 1,372,694 (19741, Lewin et al., 1975, pp. 161-175. D. Evaluation of Flame Retardants It has been pointed out (Sec. IIIA) that this review will not deal with thecomplex subject of flammability testing, nor with the correlation of laboratorytest results with fire hazards. However, in the laboratory development offlame-retardant compounds or systems, a meaningful evaluation of flame-retardant effectivenessand trends is essential to progress. Visual observationsof burning behavior are useful, but generally lack the means for quantitativeexpression and precision. Many laboratory techniques for evaluating specificproducts (e.g., fabrics) or specific flammability parameters (e.g., rate of flamespread) in specified configurations are documented in the technical literature.
CHEMICAL MODIFICATION OF POLYMERS 299 TABLE VII Examples of Flame-Retardant Compounds Used in Coatings Compound ( s) Coating type Reference Chlorendic anhydride Alkyd Cleaver, 1973. @$&To cp ca c( Chlorinated paraffin Alkyd Touval, 1972. and Antimony oxide Phosphonic acid or Intumescent F.B.Clarke Phosphates and polyol and J. W. Lyons JACS 88 4401 (1966x’ Vandersall, 1971.However, the most important tool for the laboratory evaluation of flamma-bility in polymers is the limiting oxygen index test developed at the GeneralElectric Company (Fenimore and Martin, 1966) for polymer sticks, and sincethen, adapted to a wide variety of polymeric materials and compositions, andto liquid fuels. The oxygen index of a material is the minimum percentage of oxygen in anoxygen-nitrogen atmosphere required to sustain combustion of the materialafter ignition : Oxygen Index (01) = [OZ1 x 100 [021 + “21The test is generally carried out with the sample burning downward in a can-dlelike manner, producing a gaseous diffusion flame above the polymer sur-face (Martin, 1968). Several recent reviews of the oxygen index test theory anduses (Nelson et al., 1975; Kanury, 1975; Fenimore, 1975) provide extensiveinformation on this subject, which is considered of great importance. Oxygenindex values for fibers and plastics are summarized in Tables VIII and IX.These may not be identical with values reported in technical publications forspecific compositions, because of variations in the specific composition, sam-ple preparation or geometry, or because of difficulties (melting and dripping)encountered in measuring the oxygen index of thermoplastic samples. Allow-ing for such variations, the oxygen index method provides a research tool ofexceptional consistency and reproducibility.
300 TESORO TABLE VIII Oxygen Index of Fabrics Made from Spun Yrs an Fiber (type) Oxygen Index I%O,] Acrylic (ACRILAN) 18.2 Cellulose Triacetate (ARNEL) 18.4 Cellulose Acetate 18.6 Polypropylene 18.6 Rayon (regenerated cellulose) 19.7 Cotton (greige) 20.1 Nylon (6,6) 20.1 Polyester (DACRON) 20.6 Wool (dry cleaned) 25.2 Modacrylic (DYNEL) 26.7 Polyvinylchloride (RHOVYL) 27.1 Aramid (NOMEX) 28.2 ~ ~~GFabric weight 4.8-7.0 oz/yd2. Source: Tesoro and Meiser (1970). TABLE IX Oxygen Index of Plasticsa ~~ Polymer (type) Oxygen Index [ % 0 2 1 Polyacetal 15.0 Poly (methyl methacrylate) 17.3 Polypropylene 17.5 Polystyrene 17.8 Cellulose (filter paper) 18.2 ABS Resin 18.8 Cellulose acetate 19.0 Polyethylene terephthalate 20.0 Polyaryl ether/polystyrene (NORYL) 24.3 Nylon ( 6 , 6 ) 24.3 Polycarbonate 24.9 Polyphenylene oxide 30.0 Polysulfone 38.0 Polyphenylene sulfide > 40.0 polyvinyl chloride 40.3 polyvinylidene chloride 60.0 Polytetrafluoroethylene 95.0aSources: Fenimore and Martin (1966),Isaacs (19701,Imhof and Stueben (1973).
CHEMICAL MODIFICATION OF POLYMERS 301VI. PROBLEMS IN POLYMER MODIFICATION WITH FLAME RETARDANTS The principles and approaches discussed in Sec. V have indicated somegeneral problems associated with the use of flame retardants in polymers, andsome formidable technological obstacles which must be overcome. Themagnitude of specific problems and obstacles depends on the end use, thelevel of fire resistance required, and polymer substrate considered. The mostimportant problems are briefly discussed below. A. Incorporation of Effective Amounts As a first approximation, modification of polymers to impart flame resist-ance requires larger amounts of the modifying reagent (comonomer, addi-tive, etc.) than modifications designed to impart other desirable properties.This fact has important consequences, since the effect of the added material(flame retardant) on polymer properties is considerable, generally negative,and difficult to overcome. The effect on polymer properties may cause thepolymer to fail one or more critical requirements, either in product manu-facture or in use. The problem is compounded by the inadequacy of labo-ratory test methods by which flame-retardant effectiveness of modifyingreagents can be evaluated. The minimum amount of flame retardant requiredcannot be established with precision and the effect on polymer flammabilitycan be defined only in relative terms, with reference to carefully specified testprocedures. The incorporation of effective amounts of flame retardants inpolymers without impairing polymer properties is an extremely difficultproblem. B. Retention in Use Assuming that an effective flame retardant and a viable approach to themodification of a given polymer have been identified, it is necessary to es-tablish that flame-retardant effectiveness will not be lost during the useful lifeof the polymer. This entails evaluation of the effect of environmental condi-tions which the product is likely to encounter in use (e.g., light, temperature,abrasion, etc.) and of aging. For some products (e.g., apparel textiles) thisalso includes the evaluation of durability to laundering (up to 50 times ormore) and dry cleaning. C. Environmental Effective flame-retardant compounds that can be retained adequately inpolymeric substrates in use are generally organic compounds of phosphorusand halogen. These may be structures which possess physiological activity,and may pose problems of several kinds. The compounds must be safely han-dled in industry (occupational health), and must not accumulate in theenvironment. They must not pose a health hazard in use, and should not
TESOROyield abnormally toxic degradation products when the modified polymersburn. These requirements are not clearly defined, and many compounds nowin use may have to be replaced as hazards resulting from their use are identi-fied and as new regulations are issued. The status of the controversy onenvironmental pollution by fire-retarded polymeric materials is currently un-der review. Studies of mutagenic and carcinogenic effects of a potentiallyeffective flame retardant (McCann et al., 1975), of toxic effects of flameretardants to fish (Gutenmann and Lisk, 1975), and physiological effects ofselected flame-resistant fabrics (St. John et al., 1976) are illustrative ofongoing efforts to define the magnitude of the problem. D. Cost The cost of chemical modification of a given polymer with flame retardantsincludes many components, including chemical cost of added flame retardant,processing cost of modification, cost of adjustments in manufacturing proc-esses for modified polymer, increased fabrication cost of products in whichthe modified polymer is used, and costs of quality control (flame resistance). Inevitably, consumers must pay higher prices for flame-resistant products.The costs are high initially, but decrease with improved technology and in-creased use. Since most flame-resistant polymers in use at this time haveneither “matured’ technologically, nor reached maximum volume usage,current economic appraisals are tentative.E. Flammability, Smoke Evolution, and Toxicity of Combustion Products Modification of polymers with flame-retardant compounds is designed todecrease the probability of ignition and of sustained combustion on exposureto heat. This is an important aspect of fire hazard. Other aspects includesmoke evolution (which can impair visibility and egress), and the formationof degradation products, either particulate or gaseous, which may be toxicor lethal. Evolution of smoke and toxic degradation products from materialsexposed to fire is a complex function of composition and of the conditions ofburning: the presence of flame retardants in the material may, in someinstances, increase smoke and toxicity of degradation product, but generali-zations are not possible on the basis of knowledge available at this time.Furthermore, laboratory tests for the evaluation of smoke evolution and oftoxicity of degradation products are of limited value in predicting the be-havior of the materials under realistic use conditions. The state of the artmust be advanced significantly before the interrelationship of flame retar-dation, smoke evolution, and toxicity can be discussed. W. POLYMERS AND APPLICATIONS Modification of polymers with flame retardants can be discussed with ref-erence to the chemical structure of the polymer to be modified (e.g., cellu-
CHEMICAL MODIFICATION OF POLYMERS 303lose, polyacrylonitrile, etc.), the major application of the polymers (e.g.,fibers, plastics, foams, etc.), or the chemistry of added flame retardants (e.g.,phosphorus compounds, halogen compounds, etc.). Each method of classifi-cation has advantages. Emphasis on polymer science and engineering requiressome combination of the first and second breakdown of the subject matter.The matrix given in Table X includes the major subject matter of this review(fibers, thermoplastic resins, and foams), but does not include thermosettingresins, elastomers, and coatings which are treated only briefly in the article. TABLE X 1 Wood I (Textile) Fibers Plastics (Thermoplastic) Cellular Plastics (Foams)CelluloseCellulose estersPolypeptidePolyamidePolyesterAcrylic ~Polyvinyl ChloridePolyolefinsPolyurethanes I I - 1PolystyrenePolyacetalPolycarbonate I Generally speaking, thermosetting resins are less likely to require modifi-cation with flame retardants than thermoplastics, and the state of the art isaccordingly less advanced. Flammability and flame retardation of elastomershave not been studied extensively to date. In the case of coatings, the subjectrequires consideration of a highly specialized technology, in which knowledgeof coating formulations is an essential component: coatings of reduced flam-mability would be treated as special formulations rather than as modifiedpolymers. There are numerous uses of polymeric materials where modification of thepolymers with flame retardants is of interest and concern as improved firesafety becomes increasingly important. In some instances, flame retardantsmust be used to meet existing flammability standards (federal, state, or local);in others, they are used to comply with performance requirements specifiedby the user; in other instances, the use of flame retardants is contemplated for
304 TESORO TABLE XI Regulations and Standard: f o r Po 1ymer i c Flanunabi t y ( 1 9 7 6 ) Material Application . In effect Planned Wood 1. Structural 2. Furnishings Fibers 1. Apparel 2. Furnishings general institutional aircraft ground t r a n s p . 3. Tents Plastics 1. Building 2. Furniture 3. Aircraft 4. Ground T r a n s p o r t a t i o n 5. Recreational Foams 1. Furnishings 2. Building 3. Aircraft 4. Ground T r a n s p o r t a t i o nfuture developments. Table XI summarizes major applications of polymericmaterials for which modification with flame retardant is now required, and/orexpected to become an important part of future technology. The building in-dustry, and the transportation industry (aircraft and ground transportation)will probably consume large volumes of flame-resistant (modified) polymersas new flammability standards and regulations are promulgated. Vm. WOOD, BOARD, AND PAPER The importance of wood and wood-based products (insulation board, hard-board, and particle board) in our environment is obvious. Similarly, enor-mous quantities of paper and paperlike products are consumed daily,frequently in situations where fire safety considerations are important. Woodand paper products consist essentially of cellulose, as do the cellulosic textilefibers to be discussed in a later section of this review. Thus, flame-retardantcompounds that inhibit flammability of cellulose are, in principle, effectivefor wood, paper, and cellulosictextiles. It is clear, however, that flammability
CHEMICAL MODIFICATION OF POLYMERS 305and performance requirements, durability of flame resistance, critical side ef-fects, and economics are vastly different for these products. The subject offlame retardants for cellulose must be divided into its logical components;namely, wood and wood-based products, paper products, and cellulosictextiles. A. Wood Products Modification of wood and wood-based products with flame retardants aimsat preventing ignition and at reducing the rate of flame spread if ignition oc-curs. It can be approached either by impregnation of the substrate with flameretardants, or by surface coatings. The former method has a long history,dating back to the first century B.c., when alum and vinegar solutionswere used as fire-retardant treatments for wood ! Nevertheless, only aboutsix million cubic feet of wood and plywood were treated with flame retardantsin 1972-less than 0.1 % of the annual production! The cost of treatment hasbeen the principal reason for such limited use. Although the flame-retardantchemicals are relatively inexpensive, the processing cost is high and thetreatment increases the cost of the wood or wood products by 50-100%. Thechemicals and treatment processes used commercially (Eickner, 1966) havebeen developed primarily from empirical knowledge and pragmatic obser-vations over the years. Recent research on the manner in which flame-retard-ant compounds alter pyrolysis and combustion processes in wood cellulosenow provides a conceptual framework for established approaches and for newdevelopments as well. It is now generally accepted that flame-retardant chemicals that are effectivefor cellulose (specifically wood) alter the course of thermal degradation reac-tions in the solid phase, increasing the amount of char, water, and carbondioxide formed at the expense of combustible degradation products (organicvolatiles-tars and gases). Evidence for this mechanism of effectiveness hasbeen obtained primarily by thermal methods of analysis. A review of theliterature on thermal degradation of wood components (Beall and Eickner,1970) coupled with the results of investigations carried out on wood treatedwith flame retardants (Tang and Eickner, 1968; Lyons, 1970a) have estab-lished that effective flame retardants facilitate degradation reactions. Volatiledegradation products from treated wood provide less energy on combustionthan the same weight of volatiles from untreated wood, while the char yield issignificantly increased. Thermal data showing the effect of additives in alpha-cellulose (Tang and Neil, 1964) are shown in Table XII, and are indicative ofthe approaches used for imparting flame resistance to wood, involving pri-marily inorganic salts. A summary of inorganic salts which have been foundeffective is presented in Table XIII. Eickner (1966) points out that these inorganic salts are generally used inmixtures containing several compounds (e.g., 10 parts diammonium phos- + +phate 60 parts ammonium sulfate + 10 parts borax 20 parts boricacid = “Minalith formulation”). Aqueous solutions containing 12-1 5 %
306 TESORO TABLE Xn Thermal Data for a-CelluloW Activation Max rate energy of, Heat of of heat pyroiysis.. pyrolysis generation Additive Kcal/mOle cal/g cal/g/min I None 33-35 88 870 2% NazB407 10 H z O 30-32 58 730 2% A1CEs 6H2O 33-33.5 57 665 2% KHC03 19-21 72 588 2% N H ~ H ~ P O I , 17-19 78 635 8% NHbH2POs --- 64 490#After Tang and Neil, 1964.*First stage, zero to first order.concentrations of the flame-retardant salts are used for pressure impregnationof lumber or plywood, aiming for a dry-salt retention of 2.5-3 lb/ft3 forplywood or 2-in. lumber (and decreasing amounts for thicker lumber). Similar formulations can be used for the treatment of fiber board and hard-boards. The pulp may be treated before sheet formation, or the wet pressedmat may be treated before drying. Hardboards have also been treated by pres-sure impregnation after hot pressing. Related processes have been disclosedfor particle board (Lewin et al., 1975). Approaches for chemical modification of wood with organic and/or reac-tive flame-retardant compounds include (1) impregnation from emulsions oforganic phosphates in combination with oil-borne preservatives (Gooch etal., 1959); (2) impregnation from solvent solution of organic compounds ofphosphorus and halogen (Lyons, 1970a; Lewin et al., 1975); (3) impregnationwith (unsaturated) organophosphorus monomers polymerized i situ by nradiation (Raff et al., 1966); (4) bromination of lignin to produce bromolig-nin as the effective flame retardant (Lewin et al., 1965). To date, these approaches are developmental at best, and no commercialutilization has been reported, presumably due to the high cost of the chemicalsand/or processes needed. Modification by impregnation from aqueous solu-tions of reactive flame-retardant compounds, followed by i situ insolubiliza- ntion, either by reaction with cellulose hydroxyls or by polymerization, is notpractical for the treatment of wood (even though it is the method of choicefor the treatment of cellulosic textiles). Since insolubilization of the reactivesystem is generally brought about by heat-curing, the thickness of the woodsubstrate prevents the rapid uniform temperature distribution which is read-ily attained in the case of thin sheets such as textiles. Wood and wood-based products properly treated with fire-retardant formu-
CHEMICAL MODIFICATION OF POLYMERS 307 TABLE XI11 Compound ( s ) ReferencesNHs HzPOI, R. H. Mann et al., (NHs)2HPOs Proc. Am. Wood Preservers (NHs)2S01, ASSOC. (1944), 261,with and without T R. Truax et a l . , . addition of urea o r Proc. Am. Wood Preservers other components Assoc. (19331, 107. G. M. Hunt et al., Proc. Am. Wood Preservers ASSOC. (1932), 71. ZnC&2 + H. W. Angell, Na2Cr207 * 2H20 Proc. Forest Products Res. SOC. - 107 (1951). 5, D. F. McCarthy et al., J. Inst. Wood Sci. 5 (I), 24 (1972).lations have decreased rates of surface flame spread (ASTM Test for surfaceburning characteristics of building materials E-84-61) and are self-extinguish-ing (flaming and glowing) when the external source of heat is removed. Thefire-retardant treatments also reduce the maximum rate of heat release. Theamount of smoke produced by burning the treated wood depends greatly onthe chemicals included in the formulation and on the fire exposure conditions.Information about the effects of treatment on the toxicity of the pyrolysis andcombustion products is very limited. Untreated wood produces some toxiccarbon monoxide and irritant gases and vapors, such as acetic acid, formal-dehyde, glucosans, and phenols in burning. The use of fire retardants resultsin a reduced percentage of tars and vapors and in a greater percentage of woodretained as a charcoal residue. In modifying wood by chemical treatment, the influence on many proper-ties must be considered, including the effect of added flame retardants on
308 TESOROstrength, durability, hygroscopicity, corrosiveness, painting, gluing, and ma-chining characteristics. Reduced performance in some of these characteristics(in addition to the cost of fire-retardant treatment) has limited the use ofwood-based products treated with fire retardants. Many of the chemicals used as fire retardants are water-soluble inorganicsalts, easily leached from the wood : therefore, the treatments are primarilylimited to interior uses. Furthermore, some chemicals used in fire-retardant formulations are hy-groscopic, and as water is absorbed, droplets may come to the surface anddrop from the treated substrate, with consequent loss of fire retardant. Manyof the inorganic salts used as fire retardants are corrosive to certain metalsand alloys. Formulations can be balanced and neutralized, and commercialcorrosion inhibitors added so that this does not pose a problem. However,if treated wood is exposed for long periods at high relative humidities, mois-ture and chemicals may be exuded on the metals, and produce various formsof electrolytic corrosion, which the inhibitors may not be able to control. The processing and addition of fire-retardant chemicals to wood decreasethe modulus of elasticity by 5-10%, and the modulus of rupture by 1620%as compared to untreated controls. There is also a decrease in resistance toimpact loading. Additional problems to be considered in the evaluation of wood treatedwith fire retardants are the possible abrasive effect of the salts present on cut-ting tools (machining); the effect of the additive on adhesive bonding of struc-tural components (gluing), and of surface coatings (painting). B. Paper Products Flame retardants recommended for paper and paper products have closelyparalleled those suggested for other forms of cellulose, particularly wood,since the beginning of this century. The most commonly used materials areammonium sulfate and ammonium phosphates, with or without boric acid,but a large number of more sophisticated retardants have been suggested forvarious specialty applications (Lyons, 1970a).There are several modes of add-ing flame retardants to paper products, depending on the solubility of thecompounds, on the paper product involved, and on cost considerations. Theselection and application of specific flame retardants to paper products as afunction of the inherent specialized technology are considered beyond thescope of this review. M. FIBERS AND FABRICS A. Cellulose (Cotton and Rayon) 1. Introduction There are important historical and economic reasons for the fact that the
CHEMICAL MODIFICATION OF POLYMERS 309science and technology of flame retardants for cellulose fibers are far moreadvanced than for other fibers and polymers: until perhaps 25 years ago, anoverwhelming proportion of all textiles used was made of cellulosic fibers,and until recently the research challenge of reducing flammability in poly-mers has focused primarily on wood (Sec. VIII) and on cotton as the sub-strates. The classic textbooks of the 1940s on the subject of flame retardantsfor fabrics (Little, 1947; Ramsbottom, 1947) thus cover cellulosics exclu-sively. Extensive research on the thermal degradation of cellulose (Shafizadeh,1968) and on the manner in which added flame retardants alter the course ofdegradation reactions, has led to a partial elucidation of the mechanism offire-retardant action by Lewis acids. The principal role of acid or acid-form-ing flame retardants in cellulose is to enhance dehydration and char for-mation in the condensed phase, suppressing the formation of combustiblevolatiles in the thermal degradation process. This theory, first postulated manyyears ago (Schuyten et al., 1955), has been supported by experimental evi-dence obtained on many cellulosic substrates and flame-retardant compounds.Phosphorus acids are particularly efficient in catalyzing cellulose dehydra-tion, and phosphorus-containing flame retardants have been studied mostextensively. In the case of natural cellulosic fibers, modification with flame-retardant compounds has been accomplished almost exclusively by finishingof fabrics. In the case of regenerated cellulose fibers, the most important ap-proach to modification has been the incorporation of flame-retardant addi-tives in the spinning fluid (see Sec. VC). 2. Cotton Fabrics Flame-retardant finishes for cotton fabrics have been reviewed in books(Little, 1947; Lyons, 1970a; Lewin et al., 1975), encyclopaedia articles(Drake, 1966,1971), and in a large number of other publications. Literally hun-dreds of formulations, and dozens of different compounds have been proposed.Milestones of the evolution from simple processes involving deposition of in-organic salts (readily removed by water) to sophisticated modifications of thecellulose molecule and/or in situ polymerization of appropriate monomersare summarized in Table XIV. The most significant relevant references areindicated at the end of Table XIV. The definition of “ideal” requirements for durable flame retardants forcotton fabrics was perfectly formulated by Sir William Perkins in 1912 (Ref.2 in Table XIV; see also Lyons, 1970a). Perkins’ attempt to precipitate a water-soluble flame-retardant compound (stannic oxide) in situ to attain durabil-ity to laundering remains an important conceptual milestone in the evolu-tion of current technology. Methods for testing flame resistance of treatedcottons were crude and pragmatic. They were not formalized until interestin the treatments was stimulated by the military in the late 1930s. During theperiod of World War 11, a vertical flammability test was developed for fabricstreated with flame retardants (ASTM-D-626 ; AATCC 34 ; Federal Spec.
310 TESORO TABLE XIV History of Flame Retardants for Cellulosic Fabrics Year Compounds Applications Ref. 1821 Mixtures of ammonium Linen and jute fabrics (1) phosphate, ammonium chloride and borax 1912 Sodium stannate Cotton flannel (2) followed by ammonium sulfate to precipi- tate stannic oxide in situ-1940 Chlorinated paraffin Canvas for military (3) and antimony oxide tentage "FWWMR" finish-1948 Phosphorylation of Cotton fabrics cotton (urea- for apparel phosphate) Titanium oxychloride Cotton fabrics and antimony oxy- "ERIFON" finish chloride 1956- Trisaziridinyl phos- All types of 1958 phine oxide (APO) cotton fabrics and Tetrakis hydroxy- methyl phosphonium chloride (THPC) devel- oped at USDA as com- ponents of durable finishing systems 1968- N-methy lo1 dimethy1 All types of 1969 phosphonopropion- cotton fabrics amide (Pyrovatex CP) 1969- N,N,N" Trimethyl All types of 1970 phosphoramide with cotton fabrics trimethylol melamine (MCC 100/200/300) 1971 Vinyl phosphonate All types of cotton (9) oligomer (Fyrol 76) fabrics copolymerized with N-methylol acrylamide 1974- Methyl phosphonic All types of cotton (10) 1975 diamide, chloromethyl fabrics phosphonic diamide Gaylussac (1821). 2Perkins (1913a, b). 3Chase (1943) and USP. 2,299,612. 4Davis et al. (1949); Nuessle (1956); and USP 2,935,471 (1960) to Dupont. 5Gulledge and Seidel (1950). GReevesandGuthrie(1956); Drake and Guthrie(1959); see also Lyons(1970a),pp. 174-178 and 189-208. 7Aenishanslinet al. (1968, 1969); and USP 3,423,369 (1969) to CIBA, Ltd. WSP 3,632,297 and 3,681,060 (1972) to J.P. Stevens. gEisenberg and Weil (1974).OTesoro, Valko, and Olds (1976).
CHEMICAL MODIFICATION OF POLYMERS 311 Decomposition ..1- Ignition /. . Non-f laming Flame Physical Response: Degradation Propagation Shrinkage, Melting Charring 8 I , I t I I oxidizer 1 Combustible gases > - Flame Non combustible gasespolymer >. - (partially decomposed polymers) olids (carbonaceous residues or char) Smoke (entrained solid or liquid particles)Fig. I . Thermal degradation, ignition, and combustion processes for organic polymersrepresented by general sequences. Thermally induced decomposition clearly precedesignition.5902, 5903) and widely adopted as a measure of flame resistance by workersin the field. Fabrics which are self-extinguishing in this test were designatedas “flame resistant” in publications from about 1940 until about 1970, whenmodifications of this test became a part of federal standards (e.g., DOC-FF-3-71). In the late 1930s and early 1940s, flame-retardant finishes based onchlorinated paraffins and antimony oxide in conjunction with resin binderswere developed for tent fabrics (Ref. 3 in Table XIV). Large amounts of fin-ish (up to 60% solids applied based on fabric weight) were used, impairingthe flexibility and air permeability of the treated fabrics. However, the finishsucceeded in combining flame resistance, water and mildew resistance for acritically important application, and 700 million yards of fabric were pro-cessed with it during World War 11. Clearly, the development was not ap-plicable to apparel fabrics. Attempts to obtain durable flame resistance in cotton by chemical modi-fication of the cellulose molecule were made in the late 1940s. Work on phos-phorylation of cellulose in the presence of large amounts of urea or other basiccompounds to prevent acid degradation and depolymerization of the poly-
312 TESOROmer (Ref. 4 in Table XIV) led to a process which was used on a commercialscale for a time. However, the phosphate ester linkage introduced into the cel-lulose is not sufficiently stable to hydrolysis to withstand repeated launderingand the presence of ion exchange sites in the modified cotton leads to replace-ment of NH: by metal cations with loss of flame resistance. Work on the reaction of cotton with titanium oxychloride and antimonyoxychloride (Ref. 5 in Table XIV) enjoyed a brief period of intense interestin the 1950s and was presumably abandoned due to practical difficulties ofhandling in the mills. The development of “modern,” truly wash-resistant, or durable flame-re-tardant finishes for cotton fabrics began in the late 1950s with the USDA in-vestigations focusing on the reactions of two organophosphorus molecules,APO and THPC (see below) - - CHz - CHz CHzOH + I HOCHz - P - CHzOH C II- I CHzOH APO THPCwith cellulose, with coreactants, and with each other (Ref. 6 in Table XIV).Self-extinguishing cotton fabrics of reasonable properties found to withstanda large number of wash cycles and exposures were obtained for the first time.During this period, two important working hypotheses evolved: that about3 % insolubilized phosphorus was needed to attain satisfactory flame resist-ance (self-extinguishing behavior in the AATCC vertical test) in most cottonfabrics; and that insolubilization of the phosphorus could be attained eitherby reaction with cellulose OH groups (e.g., phosphorylation, APO, etc.),or by in situ polymerization of appropriate monomer systems (e.g., THPCwith nitrogen-containing comonomers such as urea, NH3, etc.). Subsequentdevelopments confirmed and refined these working hypotheses. Finishes basedon THPC chemistry have been produced commercially for a decade, andremain important. Finishes based on APO chemistry have been abandonedprimarily because of toxicity and/or suspected carcinogenic properties of thereagent (APO) and its precursor (ethylene imine). Flame-resistant cotton fabrics produced commercially in the 1970s aremade by finishing with systems summarized in Table XV (reference numbersfrom Table XIV are repeated). Others have been considered, or are currentlyunder consideration: the N,N,‘N”-trimethyl phosphoramide system (Ref.8 in Table XIV) has reportedly been shelved, and the methyl phosphonic dia-mide system (Ref. 10 in Table XIV) has not reached commercial status.
TABLE XV Commercial Chemicals for Flame-Retardant Finishing of Cotton Fabrics Organophosphorus Coreactant (s) Insolubilization % Finish %p a Compound Required (Ref) Applied Insol. Insol. 0 /I (CH30)2 P-CHZCH2CONHCH20H - -- Reaction with 30-40 20-30 2- 3 c e l l u l o s e OH * NH3, In s i t u 30-40 25-35 3-5 [ (HOCH2) sPI + X- polycondensa- X = CL, OH, e t c . NH2CONH2, etc. tion CH 2= CH CO N H CH 20H In s i t u 25-35 20-30 2-4 polyaddition ;H=CH (free radical polymerization)aFor SE behavior in vertical flammability tests.bAenishanslin et al. (1968, 1969) and USP 3,423,369 (1969) to CIBA, Ltd.CReeves and Guthrie (1956); Drake and Guthrie (1959). See also Lyons (1970a).dEisenberg and Wed (1974). k! w
TABLE XVI Experimental Chemicals for Flame-Retardant Finishing of Cotton Fabrics Organophosphorus Coreactant (s) Insolubilization % Finish a % P Compound ( %P) Required Mechanism Insolubilized Insol. S NH ~r O 3 N H 2 Reaction w i t h 15-20 2.0-2.2 + c e l l u l o s e OHb ( + 2% S ) b i s methoxy- m e t h y l uron Reaction w i t h 8-16 2.0-3.1 c e l l u l o s e OH (17.2) Reaction with 7-14 1.8-3.6 c e l l u l o s e OH (33.0)aFor SE behavior in vertical flammability tests.bLewin et al. (1973).CTesoro, Olds, and Babb (1974).dTesoro, Valko, and Olds (1976).
CHEMICAL MODIFICATION OF POLYMERS 315 Table XVI summarizes experimental chemicals of continuing interest atthis time. 3. Other Cellulosic Fabrics In principle, approaches used for finishing of cotton fabrics are applicableto other cellulosics (rayon, linen, jute, etc.). In fact, the properties of differ-ent fibers and fabrics require extensive modifications in the technology of theprocess, and in the amounts of flame-retardant finish needed to attain a speci-fied level of flame resistance. A discussion of these differences from the view-point of textile technology is beyond the scope of this review. Suffice it to saythat commercial production of flame-resistant 100% cellulosic fabrics byfinishing has been limited to cotton, and some specific rayon fabrics (e.g.,draperies). 4. Regenerated Cellulose (Rayon) Fibers The incorporation of flame-retardant additives in the fiber-spinning processis a problem of considerable complexity. The technical accomplishment ofhaving developed and produced flame-resistant rayon fiber on a commercialscale should not be underestimated. Whatever the commercial future of thisproduct may hold, its development can be considered an important milestonein fiber technology. Flame-resistant rayon fiber can be used to manufacture fabrics which areself-extinguishing in a vertical test. It has been made commercially by incor-porating an alkoxyphosphazene in the spinning fluid (Fig. 3). The commercialfiber employs the n-propoxy compound (R = n-C3H7-) as the additive(Godfrey, 1970): RO OR P N N NOther approaches in which the rayon fiber is modified by graft copolymeriza-tion reaction with a flame-retardant monomer prior to yarn manufacture(Krassig, 1970; Brickmann and Faessinger, 1973) have been suggested, buthave not reached commercial status to date. Appreciable quantities of disposable nonwoven textile items are produced
316 TESOROfrom rayon. These are not generally laundered for re-use and if flame resist-ance is needed, the materials can be treated with water-soluble inorganic flameretardants such as diammonium phosphate or ammonium sulfamate inappropriate formulations. B. Cellulose Acetate and Triacetate Cellulose acetate and triacetate fibers, or cellulose ester fibers made by ace-tylation of natural cellulose, are thermoplastic. They melt at relatively lowtemperature (Mark et al., 1968), they ignite, and they can propagate the flameeven though they drip while they continue to burn. The principal, or perhapsthe only method used to attain fire resistance in cellulose acetate and triace-tate fibers is the incorporation of a flame-retardant additive (specifically, 2,3tris dibromopropyl phosphate) (LeBlanc et al., 1973) into the spinning solu-tion before extrusion. The bromine-containing product (flame-resistant ace-tate) obtained is somewhat more resistant to ignition than the unmodifiedacetate. Above all, if ignited, the modified material tends to drip without sus-taining flame propagation and it is rated as self-extinguishing in vertical testsproviding it is not tested or used in conjunction with a nonthermoplastic ma-terial (e.g., thread). If a nonthermoplastic component is present in the sys-tem, it acts as a wick for the molten acetate or triacetate polymer and burningis sustained. In this case, the amount of flame-retardant additive commonlyused in spinning (about 10 % based on polymer weight) is not sufficient to im-part flame resistance and self-extinguishing behavior. Larger amounts of addi-tive, on the other hand, would impair fiber properties and therefore not bepractical. C. Wool and Protein Fibers Although the unique chemical structure of wool and other protein fibersoffers many reaction sites and possibilities for chemical modification, studiesof flame retardants in wool have been limited in number and in scope. Thereasons are clear, since wool consumption is a very small percentage of totalfiber consumption and, furthermore, wool textiles are generally less flam-mable than those made from cotton, regenerated cellulose, or from most syn-thetic fibers. While most wool fabrics would not be self-extinguishing in vertical flam-mability tests, wool has a relatively high oxygen index and it exhibits relativelylow flammability in tests less stringent than the vertical test. Work designedto enhance the “natural” flame resistance of wool has been reviewed by Be-nisek (Benisek, 1972, 1973; Lewin et al., 1975) . Modification of wool with flame retardants has been based on three ap-proaches: (1) nondurable treatments, mainly inorganic borates or phos-phates, applied to fabrics for specialized applications such as theater curtainsor aircraft upholstery; (2) modifications of systems developed for cellulosicsand based on THPC chemistry, primarily developed to meet aircraft uphol-